1.
Chapter 7 Deformation and strengthening mechanisms
2.
Why study deformation and strengthening mechanism? <ul><li>Most of metallic products are produced through deforming the metal somehow to obtain desired shape, size and strength. But what factors would influence the process of deformation? </li></ul><ul><li>You may have an experience that an iron wire will get tougher and it will break finally when it is bended for times. Do you know why? </li></ul><ul><li>Study on deformation and strengthening mechanism will help us use and develop materials better. </li></ul>
3.
What should you be able to do after studying this chapter? <ul><li>Describe dislocation motion from an atom’s perspective. </li></ul><ul><li>Understand the relationships between dislocation motion and plastic deformation of metallic materials. </li></ul><ul><li>Define slip system and explain the influence of slip system on the deformability of materials. </li></ul><ul><li>Explain mechanism of grain boundary strengthening, solid-solution strengthening, strain hardening. </li></ul><ul><li>Describe recovery and recrystllization in terms of both the alternation of microstructure and mechanical characteristics of the material. </li></ul>
4.
Important terms and concepts: <ul><li>Cold working 冷加工 </li></ul><ul><li>Critical resolved shear stress 临界分剪切应力 </li></ul><ul><li>Dislocation density 位错密度 </li></ul><ul><li>Grain growth 晶粒生长 </li></ul><ul><li>Lattice strain 晶格应变 </li></ul><ul><li>Recovery 回复 </li></ul><ul><li>Recrystallization temperature 再结晶温度 </li></ul><ul><li>Resolved shear stress 分剪切应力 </li></ul><ul><li>Slip 滑移 </li></ul><ul><li>Slip system 滑移系 </li></ul><ul><li>Recrystallization 再结晶 </li></ul>
6.
Key knowledge points: Deformations mechanisms for metals <ul><li>1. Historical: </li></ul><ul><li>1930s, theory and actually measured discrepancy in mechanical strengths </li></ul><ul><li>1950s, dislocation be examined by electron microscope </li></ul>
7.
2. Basic concepts of dislocations <ul><li>Plastic deformation corresponds to the motion of large numbers of dislocations. </li></ul><ul><li>An edge dislocation moves in response to a shear stress applied in a direction perpendicular to its line. </li></ul><ul><li>In an edge dislocation, localized lattice distortion exists along the end of an extra half-plane of atoms. </li></ul><ul><li>The mechanics of dislocation motion are represented in Fig.7 .1 </li></ul>
8.
The mechanics of dislocation motion <ul><li>Fig.7.1 Atomic rearrangements that accompany the motion of an edge dislocation as it moves in response to an applied shear stress. </li></ul><ul><li>The extra half-plane of atoms is labeled A. </li></ul><ul><li>The dislocation moves one atomic distance to the right as A links up to the lower portion of plane B; in the process, the upper portion of B becomes the extra half-plane. </li></ul><ul><li>A step forms on the surface of the crystal as the extra-plane exists. </li></ul>
9.
<ul><li>Slip ------- the process by which plastic deformation is produced by dislocation motion is termed slip. </li></ul><ul><li>slip plane - ----the crystallographic plane along which the dislocation line traverses is the slip plane. </li></ul><ul><li>Macroscopic plastic deformation simply corresponds to permanent deformation that results from the movement of dislocations, or slip, in response to an applied shear stress. </li></ul>
10.
<ul><li>Drawing a carpet in the way of (a) and (b) may help you understand the motion of dislocation better. </li></ul>
11.
Dislocation motion is analogous to the mode of locomotion employed by a caterpillar ( Fig.7.3)
12.
<ul><li>The motion of a screw dislocation in response to the applied shear stresses shown in Fig.7.2b . the direction of movement is perpendicular to the stress direction. </li></ul><ul><li>For an edge, motion is parallel to the shear stress. However, the net plastic deformation for the motion of both dislocation types is the same. </li></ul><ul><li>The direction of motion of the mixed dislocation line is neither perpendicular nor parallel to the applied stress, but lies somewhere in between. </li></ul>
13.
Fig.7.2 The formation of a step on the surface of a crystal by the motion of (a) an edge dislocation and (b) a screw dislocation. Note that for an edge, the dislocation line move in the direction of the applied shear stress τ ; for a screw, the dislocation line motion is perpendicular to the stress direction.
14.
<ul><li>Dislocation density --------the number of dislocation in a material is expressed as the total dislocation length per unit volume, or equivalently, the number of dislocations that intersect a unit area of a random section. </li></ul><ul><li>The units of dislocation density are millimeters of dislocation per cubic millimeter or just per square millimeter. </li></ul>
15.
Dislocation density <ul><li>Solidified metal crystal 10 3 mm -2 </li></ul><ul><li>Heavy deformed metal 10 9 to 10 10 mm -2 </li></ul><ul><li>Heat treating could reduce the density to on the order of 10 5 to 10 6 mm -2 </li></ul><ul><li>Ceramic materials 10 2 to 10 4 mm -2 </li></ul><ul><li>Silicon single crystal 0.1 to 1 mm -2 </li></ul>Do you find some relationships between deformation and density of dislocation? What is it? What does it mean?
16.
3. Characteristics of dislocation <ul><li>When metals are plastically deformed, some fraction of the deformation energy (approximately 5% ) is retained internally, the remainder is dissipated (lost 消失 ) as heat. The major portion of this stored energy is as strain energy associated with dislocations. </li></ul><ul><li>Lattice strains (Fig.7.4) --- some atomic lattice distortion exists around the dislocation line because of the presence of the extra half-plane of atoms. </li></ul>
17.
Fig.7.4 Regions of compression (dark) and tension (colored) located around an edge dislocation.
18.
<ul><li>The strains extend into the surrounding atoms, and their magnitudes decrease with radial distance from the dislocation. </li></ul><ul><li>The strain fields surrounding dislocations in close proximity to one another may interact such that forces are imposed on each dislocation by the combined interactions of all its neighboring dislocations. ( Fig.7.5) </li></ul>
19.
Fig.7.5 (a) Two edge dislocation of the same sign and lying on the same slip plane exert a repulsive force on each other; C and T denote compression and tensile regions, respectively. (b) Edge dislocations of opposite sign and lying on the same slip plane exert an attractive force on each other. Upon meeting, they annihilate each other and leave a region of perfect crystal.
20.
4. Slip system <ul><li>Dislocations do not move with the same degree of ease on all crystallographic planes of atoms and in all crystallographic directions. </li></ul><ul><li>Ordinarily there is a preferred plane , and in that plane there are specific directions along which dislocation motion occurs. </li></ul><ul><li>This plane is called the slip plane . It follows that the direction of movement is called the slip direction . </li></ul>
21.
<ul><li>slip system - ------ This combination of the slip plane and the slip direction. The slip system depends on the crystal structure of the metal and is such that the atomic distortion that accompanies the motion of a dislocation is a minimum. </li></ul><ul><li>For a particular crystal structure, the slip plane is that plane having the most dense atomic packing, that is has the greatest planar density. </li></ul>
22.
<ul><li>The slip direction corresponds to the direction, in this plane, that is most closely packed with atoms, that is, has the highest linear density. </li></ul><ul><li>For example: FCC crystal structure, {111}slip plane, <110>slip direction, 12 slip system ( Fig.7.6 and table 7.1) </li></ul><ul><li>The more slip system, the more ductile of the metal. HCP metals have few active slip systems, are normally quite brittle. </li></ul>
25.
5. Plastic deformation of polycrystalline metals <ul><li>For polycrystalline metals, the direction of slip system varies from one grain to another. For each, dislocation motion occurs along the slip system that has the most favorable orientation (i.e., the highest shear stress). ( Fig. 7.10 ) </li></ul><ul><li>Gross plastic deformation of a polycrystalline specimen corresponds to the comparable distortion of the individual grains by means of slip. (Fig. 7.11) </li></ul>
26.
<ul><li>Figure 7.10 slip lines on the surface of a polycrystalline specimen of copper that was polished and subsequently deformed. </li></ul>
27.
<ul><li>Figure 7.11 Alteration of the grain structure of a polycrystalline metal as a result of plastic deformation. </li></ul><ul><li>(a) Before deformation the grains are equiaxed. </li></ul><ul><li>(b) The deformation has produced elongated grains. </li></ul>
28.
<ul><li>During deformation, mechanical integrity and coherency are maintained along the grain boundaries. As a consequence, each individual grain is constrained, to some degree, in the shape it may assume by its neighboring grains. </li></ul><ul><li>Polycrystalline metals are stronger than their single-crystal equivalents, which means that greater stresses are required to initiate slip and the attendant yielding. </li></ul>
29.
Mechanisms of strengthening in metals <ul><li>Metallurgical and materials engineers are often called on to design alloys having high strengths yet some ductility and toughness. Ordinarily, ductility is sacrificed when an alloy is strengthened. </li></ul><ul><li>Important to the understanding of strengthening mechanisms is the relation between dislocation motion and mechanical behavior of metals. </li></ul>1. Strengthening by grain size reduction （细晶强化）
30.
<ul><li>Macroscopic plastic deformation corresponds to the motion of large numbers of dislocations, the ability of a metal to plastically deform depends on the ability of dislocations to move. </li></ul><ul><li>Restriction or hindering dislocation motion renders a material harder and stronger. </li></ul><ul><li>The size of the grains, or average grain diameter, in a polycrystalline metal influences the mechanical properties. (Fig. 7.14) </li></ul>
31.
Fig.7.14 The motion of a dislocation as it encounters a grain boundary, illustrating how the boundary acts as a barrier to continued slip. Slip planes are discontinuous and change directions across the boundary.
32.
The grain boundary acts as a barrier to dislocation motion for two reasons <ul><li>Since the two grains are of different orientations, a dislocation passing into grain B will have to change its direction of motion; this becomes more difficult as the crystallographic misorientation increases. </li></ul><ul><li>The atomic disorder within a grain boundary region will result in a discontinuity of slip planes form one grain into the other </li></ul>
33.
<ul><li>A fine-grained material ( one that has small grains) is harder and stronger than one that is coarse grained, since the former has a greater total grain boundary area to impede dislocation motion. </li></ul><ul><li>Hall-Petch equation: </li></ul><ul><li>σ y = σ 0 + k d -1/2 </li></ul>
34.
2.Solid-Solution Strengthening ( 固溶强化 ) <ul><li>High-purity metals are almost always softer and weaker than alloys composed of the same base metal. </li></ul><ul><li>Increasing the concentration of the impurity results in an attendant increase in tensile and yield strengths. </li></ul><ul><li>solid-solution strengthening---impurity atoms go into either substitutional or interstitial solid solution impose lattice strains . </li></ul>
35.
<ul><li>Alloys are stronger than pure metals because impurity atoms that go into solid solution ordinarily impose lattice strains on the surrounding host atoms. </li></ul><ul><li>Lattice strain filed interactions between dislocations and these impurity atoms result, and consequently, dislocation movement is restricted. Fig. 7.16 7.17, 7.18 </li></ul>
36.
3. strain hardening or work hardening or cold working ( 形变强化，冷作硬化） <ul><li>Strain hardening is the phenomenon whereby a ductile metal becomes harder and stronger as it is plastically deformed. </li></ul><ul><li>Sometimes it is also called work hardening, or, because the temperature at which deformation takes place is ‘‘cold’’ relative to the absolute melting temperature of the metal, cold working. Most metals strain harden at room temperature. </li></ul><ul><li>It is sometimes convenient to express the degree of plastic deformation as percent cold work rather than as strain. Percent cold work (%CW) is defined as </li></ul><ul><li>where A 0 is the original area of the cross section that experiences deformation, and A d is the area after deformation. </li></ul>
37.
<ul><li>Fig.7.16 Variation with nickel content of </li></ul><ul><li>tensile strength, </li></ul><ul><li>yield strength, and </li></ul><ul><li>ductility for copper-nickel alloys, showing strengthening. </li></ul>
38.
Fig.7.17 (a) Representation of tensile lattice strains imposed on host atoms by a smaller substitutional impurity atom. (b) Possible locations of smaller impurity atoms relative to an edge dislocation such that there is partial cancellation of impurity-dislocation lattice strains.
39.
Fig.7.18 (a) Representation of compressive strains imposed on host atoms by a larger substitutional impurity atom. (b) Possible locations of larger impurity atoms relative to an edge dislocation such that there is partial cancellation of impurity-dislocation lattice strains.
40.
<ul><li>The dislocation density in a metal increase with deformation or cold work, due to dislocation multiplication ( 繁殖 , 增加 ) or the formation of new dislocations. </li></ul><ul><li>On the average, dislocation-dislocation strain interactions are repulsive. The net result is the motion of a dislocation is hindered by the presence of other dislocations. </li></ul>
41.
Recovery, recrystallization, and grain growth <ul><li>Plastically deforming a polycrystalline metal specimen at temperatures that are low relative to its absolute melting temperature produces microstructure and property changes that include </li></ul><ul><li>(1) a change in grain shape </li></ul><ul><li>(2) strain hardening </li></ul><ul><li>(3) an increase in dislocation density. </li></ul>
42.
<ul><li>Some fraction of the energy expanded in deformations is stored in the metal as strain energy which is associated with tensile, compressive and shear zones around the newly created dislocations. These properties and structures may revert (return) back to the precold-worked states by appropriate heat treatment. </li></ul><ul><li>Such restoration results from two different processes that occur at elevated temperatures: recovery and recrystallization, which may be followed by grain growth. </li></ul><ul><li>. </li></ul>
43.
Recovery <ul><li>During recovery, some of the stored internal strain energy is relieved by virtue of dislocation motion (in the absence of an externally applied stress), as a result of enhanced atomic diffusion at the elevated temperature. </li></ul><ul><li>There is some reduction in the number of dislocations, and dislocation configurations (similar to that shown in Figure 5.12) are produced having low strain energies. </li></ul><ul><li>In addition, physical properties such as electrical and thermal conductivities and the like are recovered to their precold-worked states. </li></ul>
44.
Recrystallization <ul><li>Recrystallization is the formation of a new set of strain-free and equiaxed grains that have low dislocation densities and are characteristic of the pre-cold-worked condition. (Fig. 7.21) </li></ul><ul><li>After recrystallization, the metal becomes softer, weaker, yet more ductile. </li></ul><ul><li>Recrystallization temperature ----the temperature at which recrystallization just reaches completion in 1h. Typically, it is between one third and one half of the absolute melting temperature of a metal or alloy and depends on several factors, including the amount of prior cold work and purity of the alloy. </li></ul>
45.
Fig.7.22 The influence of annealing temperature on the tensile strength and ductility of a brass alloy. Grain size as a function of annealing temperature is indicated. Grain structures during recovery, recrystallization, and grain growth stages are shown schematically.
47.
Important conclusions: <ul><li>On a microscopic level, plastic deformation of metals corresponds to the motion of dislocations in response to an externally applied a hear stress, a process termed slip. Slip occurs on specific crystallographic planes and within these planes only in certain directions. </li></ul><ul><li>A slip system represents a slip plane- slip direction combination, and operable lips systems depend on the crystal structure of the material. </li></ul>
48.
<ul><li>Since the ease with which a metal is capable of plastic deformation is a function of dislocation mobility, restriction of dislocation motion increases hardness and strength. </li></ul><ul><li>On the basis of this principle, three different strengthening mechanisms were discussed. They are grain boundaries strengthening, Solid solution strengthening and strain hardening. </li></ul>
49.
<ul><li>Grain boundaries serve as barriers to dislocation motion; thus refine the grain size of a polycrystalline metal renders it harder and stronger. </li></ul><ul><li>Solid solution strengthening results from lattice strain interactions between impurity atoms and dislocations. </li></ul><ul><li>And, finally, as a metal is plastically deformed, the dislocation density increase, as does also the extent of repulsive dislocation-dislocation strain field interactions; strain hardening is just the enhancement of strength with increased plastic deformation . </li></ul>
A particular slide catching your eye?
Clipping is a handy way to collect important slides you want to go back to later.
Be the first to comment